- Email: [email protected]

Contents lists available at ScienceDirect

Physica E journal homepage: www.elsevier.com/locate/physe

Quantum dot resonant tunneling FET on graphene Hakimeh Mohammadpour Department of Physics, Azarbaijan Shahid Madani University, 53714-161 Tabriz, Iran

H I G H L I G H T S

A ﬁeld effect transistor based on graphene nanoribbon (GNR) is modeled. The chosen GNR is semiconductor with a gap. The two ends of GNR are n-type doped and play role of the metallic reservoirs. The gate length is less than the channel length so two ends of channel are un-gated. Two un-gated regions of channel act as quantum barriers. So discrete energy levels are generated in channel and resonant tunneling transport occurs through these levels.

art ic l e i nf o

a b s t r a c t

Article history: Received 14 November 2015 Received in revised form 31 January 2016 Accepted 1 March 2016 Available online 2 March 2016

At this paper a ﬁeld effect transistor based on graphene nanoribbon (GNR) is modeled. Like in most GNRFETs the GNR is chosen to be semiconductor with a gap, through which the current passes at on state of the device. The regions at the two ends of GNR are highly n-type doped and play the role of metallic reservoirs so called source and drain contacts. Two dielectric layers are placed on top and bottom of the GNR and a metallic gate is located on its top above the channel region. At this paper it is assumed that the gate length is less than the channel length so that the two ends of the channel region are un-gated. As a result of this geometry, the two un-gated regions of channel act as quantum barriers between channel and the contacts. By applying gate voltage, discrete energy levels are generated in channel and resonant tunneling transport occurs via these levels. By solving the NEGF and 3D Poisson equations self consistently, we have obtained electron density, potential proﬁle and current. The current variations with the gate voltage give rise to negative transconductance. & 2016 Elsevier B.V. All rights reserved.

Keywords: Graphene FET Quantum dot NTC Resonant tunneling NEGF

1. Introduction Negative transconductance (NTC) has wide applications in both digital and analog electronics and has been invoked in many quantum electronic devices specially at tunneling transistors and diodes. In consideration of the NTC, nano-electronic devices beneﬁt from the quantum behavior that appears mainly due to device dimensions. Among the many devices aimed at this goal, are the graphene-based structures [1–5]. Ballistic transport of carriers in graphene in addition to its two dimensional ﬂat structure makes graphene a promising candidate for observing NTC. In previous researches the NTC has been obtained in several ways. In Ref. [1] the resonant tunneling of Dirac fermions through a boron nitride barrier sandwiched between two graphene electrodes is reported. In [6] resonant current peak in a symmetric graphene p–n layer is obtained which is controlled by chemical doping and applied gate bias. The effect is also revealed at GNR-FET with Oblique top gate http://dx.doi.org/10.1016/j.physe.2016.03.001 1386-9477/& 2016 Elsevier B.V. All rights reserved.

[7]. A large peak-to-valley ratio is reported in vertical heterostructures transistors [8]. Resonant tunneling devices based on the spin-resolved splitting of energy levels in the presence of spin– orbit interaction has also emerged [9–14]. At our previous work we have modeled a pnp-GNR-FET in which the pn barriers result in discrete energy levels and resonant tunneling current [15]. In this paper, a new GNR-FET model is proposed in which NTC due to the resonant tunneling is observed. The system is an allgraphene source-channel-drain structure sandwiched between two dielectric layers. The two ends of the GNR are highly doped and behave as reservoirs called source and drain electrodes. Two gates are located at the outer sides of the dielectric layers above the channel region. In this way, two end regions of the graphene ribbon in contact to the reservoirs are not covered by gate electrode. These layers act as barriers and give rise to discrete energy levels at the channel. The calculated current is transmitted by resonant tunneling through these levels and exhibit NTC.

92

H. Mohammadpour / Physica E 81 (2016) 91–95

2. Device model and simulation approach At this section the model device structure and physics of its function is explained. It is composed of an armchair graphene nanoribbon (A-GNR) that is sandwiched between two dielectric layers. The layers are assumed to be SiO2 with dielectric constant of about k=3.9. In this kind of FET systems the source and drain contacts as well as the channel are formed on a single graphene layer (Fig. 1). Therefore an ohmic contact between the channel and each of the reservoirs is formed and the transistor acts as traditional MOSFETs. In order to get on/off states as the main characteristics of transistor, the ribbon is required to be gap-full at the central or channel region. It is known that GNRs of zigzag-type edges do not provide energy gap and thus are practically unsuitable for usage as channel of transistor. On the other hand armchair GNRs gather semiconducting band gap in some widths of the ribbon. A-GNRs with number of unit cells in the width direction equal to NW =3m or 3m +1 (m being an integer number) reveal energy gap that increases with decreasing ribbon width (by decreasing m). At this model, as applied in many previous papers, the conducting source and drain regions are obtained by highly doping ends of the GNR [16–18]. The gate metals are separated from the ribbon above the central region by two dielectric layers. This geometry which is provided by the 2D structure of graphene and its good contact to the SiO2 layer has been used by many researches and has resonant or traditional MOSFET current-voltage characteristics depending on the parameters of system. The distinct feature of this paper that we added to the above mentioned structure is a new design of gates that give rise to resonant tunneling through the device. Here, the gate electrodes of GNR-FET (Fig. 1) cover partially the quasi-one dimensional channel at the center and leaves the two ends intact. That means the two regions of graphene channel which are connected to the source and drain are un-gated semiconductors. Hence, when the gate voltage is applied, the two ends of the channel are not affected and in this way do not provide any energy level around the Fermi energy. These ungated gap-full regions act as barriers between the reservoirs and channel region that may under suitable conditions give rise to the discrete energy levels at channel. This is the phenomenon responsible for resonant tunneling through the channel. The isolated channel at our model, gathers the quantum dot behavior by discrete energy levels. Each of the GNR reservoirs consists of 30 unit cells and the channel length, indexed by the number of one dimensional unit cells of channel, NCh (as indicated at Ref. [15]) takes different amounts. In order to obtain suitable band gap, the AGNR of width NW =9 is chosen. The charge in and current through the channel are computed by the non-equilibrium Green’s function (NEGF) formalism with nearest neighbor tight-binding Hamiltonian with an atomistic pz-orbital basis-set, self-consistently solved by the 3-dimensional Poisson equation [19]. In the real space NEGF formalism the retarded Green's function of the device is deﬁned as;

Fig. 1. Schematic representation of the MOSFET-like GNR-FET.

⎡ G (E )=⎢ (E + iη) I − H − U − ⎢⎣

⎤−1

∑ − ∑ ⎥⎥ s

d

⎦

(1)

where E is energy and U is a diagonal matrix, whose diagonal entries are the on-site potential energy and H = − t ∑i, j ci† cj is the tight-binding Hamiltonian of the simulated region where i , j stand for nearest neighbors as well as ci† and cj stand for creation and annihilation operators at sites i and j respectively. The effects of rest of the semi-inﬁnite source and drain are included through the self-energies, Σs and Σd , which are calculated according to the iterative algorithm described in [20]. η=10−5 (eV ) is assumed and t =2.7eV is the hopping energy. U is a diagonal matrix, with diagonal entries representing onsite potential energies. This matrix is obtained by self-consistent computing the charge density and the electrode potentials from the Poisson and NEGF equations. The electron density (n) is calculated from the following relation;

n=2e

∫0

+∞

dE n G (E ) 2π

(2) in

in

where G n (E )=G ∑ G† is called electron correlation function. ∑ represents the in-scattering function of the contacts and is determined by; in

∑

(E )=Γs (E ) fs (E )+Γd (E ) fd (E )

† Γs (d)=i ( ∑s (d) − ∑s (d)

(3)

) represents channel level broadening due to

the source (s) and drain (d) contacts and fs (d) (E ) are Fermi energies at contacts. The retarded Green's function G (E ) is calculated from relation (1) in which, the potential matrix, U , is required. To this end ⎯⎯⎯⎯→ → Poisson equation in the form ∇ . (Kε0 ∇U )=n (r ⃗ ) e2 should be solved which demands knowledge of the function n (r ⃗ ) in the channel. In this equation ε0 is the permittivity of vacuum and the dielectric constant K is 3.9 and e is the electron charge that in electron-volt unit equals to 1. So, a self-consistent procedure is required for obtaining n and U . Starting from an initial guess for the potential energy proﬁle, the Green's equation is solved and the resulting electron density is fed into Poisson equation for obtaining new U . This cycle is repeated until the self-consistency for U and n is achieved. After the self-consistency is achieved and the desired Green’s function is obtained the current within the device is calculated by;

I=

2e ℏ

+∞

∫

dET (E ) ( fs (E )−fd (E ) ), T (E )=trace [Γs G Γd G†]

−∞

(4)

where T ̅ (E ) is the transmission function. 2.1. Discussion The promised resonant tunneling current (at small bias voltages) stem from discreteness of the energy levels at channel. This is due to the conﬁnement restriction on the channel by the lateral barriers in contact to the reservoirs. Different parameters of the device contribute to the channel characteristics. It is evident that the larger energy level separation results in better performance of the resonant tunneling devices such as resonant tunneling transistors (RTT) , resonant tunneling diodes (RTD) and their high frequency applications. To this end the ribbon energy gap ( Eg ), which is determined by the ribbon width (NW ), separating barriers widths ( LBarrier ), doping concentration of the reservoirs in molar units ( doping ), the gate length ( L Gate ,) and the channel length ( L Ch ) which contains the whole un-doped regions between two reservoirs (such that L Ch=L Gate+LBarrier ) are involved. At the next section, the results are declared.

H. Mohammadpour / Physica E 81 (2016) 91–95

93

3. Results and discussion Let’s ﬁrst recall the parameters that are not introduced yet. LS, D are the source and drain lengths that are incorporated in Poisson equation and are assigned equal sizes at this paper. LDiel. stands for width of each of dielectric layers in the direction normal to the graphene layer. VG and VD are the gate and the drain voltages, respectively, measured with respect to the pre-assumed grounded source. We note that all the length characteristics of the device along the ribbon are presented in terms of the number of unit cells as well as in all the diagrams we take NS (D)=30 (in terms of the number of unit cells) by which the ﬂat band condition at the two far ends of reservoirs are guaranteed. Unit cell of an AGNR as depicted at [15] contains a rectangle that contains a Benzene ring at the length direction and extended in the width direction to contain all the rings at that direction, so that the ribbon may be assumed a one dimensional chain of this rectangular unit cells. The ﬁrst system that is considered has the following parameters: L Ch=40,LBarrier =5, LDiel.=2 nm,doping=0. 02,NW =9,Eg ≈0. 96 eV . The edges of the conduction and valence bands are plot after self-consistent procedure for these parameters at Fig. 2. To illustrate the gate effect on the depth of constructed quantum dot at the channel between the barriers, potential proﬁle is plot for two VG s in Fig. 3. The I − VD graphs for different amounts of VG are depicted in Fig. 4. The calculated step-like I − VD diagram is due to the discreteness of the channel energy levels which is the characteristic behavior of resonant tunneling devices. By investigating the diagrams, the non-uniform behavior of the current by for different gate voltages VG in a typical small VD is pronounced. To track this behavior, we have calculated I − VG for some values of VD and plot the results at Fig. 5. Besides the overall increase of the current the oscillations with the gate voltage is the expected behavior of this research. Hence, the negative transconductance at some voltages with peak to valley ratio (PVR) of about 3 are obtained. The strength of the level discreteness and so PVR, are determined by the isolation quality of the channel quantum dot. In this way the barriers' length as well as the channel length for a determined width play major roles. The above calculations are repeated for L Ch=50 and the corresponding diagrams are plot in Figs. 6 and 7. To investigate the effect of LBarrier , the resultant current

Fig. 3. Potential proﬁle for VG=0. 5V, 0. 8V. The depth of quantum well increases by VG .

Fig. 4. The I −VD curves for various VG s. The rise of pronounced current for VG≥0.6 (V ) and step-like increase of current are observed.

Fig. 5. I − VG for typical amounts of VD . The larger PVR at smaller VD are observed.

Fig. 2. The conduction (top) and valence (bottom) band proﬁles along the channel for the assigned voltages. The semi-Fermi levels are shown in dashed lines. (For interpretation of the references to color in this ﬁgure legend, the reader is referred to the web version of this article.)

calculated for LBarrier =7 and L Ch=40 is presented at the following section. The conduction and valence bands proﬁles along the channel are plot at Fig. 8.

94

H. Mohammadpour / Physica E 81 (2016) 91–95

Fig. 6. I − VD curves for L Ch=50 and various VG s.

Fig. 7. I − VG curves for L Ch=50 and various VD s.

Fig. 8. The conduction and valence bands along channel for assigned voltages and the same parameters of Fig. 2 for LBarrier =7, L Ch=40.

The I − VD curves for different amounts of VG are plot at Fig. 9 and the I −VG for some values of VD are plot at Fig. 10. At this point we show the discrete channel levels by considering local density of states. In Fig. 11 the density of states color plot is presented along channel as a function of energy for

Fig. 9. The I −VD curves for various VG s for L Ch=40,LBarrier =7.

Fig. 10. The I −VG curves for various VD s for L Ch=40,LBarrier =7.

Fig. 11. The density of states along channel for different energies. (For interpretation of the references to color in this ﬁgure legend, the reader is referred to the web version of this article.)

VG=0.8 (V ) and VD=0. For completeness let us show the transmission function, T(E), color plot versus the gate voltage and energy. In Fig. 12 the

H. Mohammadpour / Physica E 81 (2016) 91–95

95

the channel layer. In this way two barriers are constructed at the contact between the reservoirs (source and drain) and the channel. This conﬁnement of the semiconductor channel by the barriers forms a quantum dot channel and hence gives rise to discreteness of energy levels. The calculated current that is established by resonant tunneling through the discrete energy levels manifests NTC.

Acknowledgment This research is supported by Iran National Science Foundation (INSF), Number 9203633.

References Fig. 12. T(E) as a function of the gate voltage and energy for L Ch=40,LBarrier =7. (For interpretation of the references to color in this ﬁgure legend, the reader is referred to the web version of this article.)

horizontal axis is gate voltage and the vertical axis is energy. The transmission function at discrete energies for gate voltages above some threshold is observed which more clariﬁes the source of NTC. The minimum of the energy at which transmission occurs is shifted towards low energies by increasing the gate voltage which is a manifestation for increasing the depth of the quantum well by the gate voltage.

4. Conclusion A new design for GNR-FET is modeled in which against to the traditional GNR-FETs the gate metals cover just the middle part of

[1] L. Britnell, R.V. Gorbachev, A.K. Geim, et al., Nat. Commun. (2013) 1794. [2] G. Fiori, IEEE Electron Device Lett. 32 (2011) 1334–1336. [3] V.N. Do, A.V.H. Nguyen, P. Dollfus, et al., J. Appl. Phys. 104 (6) (2008) 0637081–063708-7. [4] Dragoman, M. Dragoman, Appl. Phys. Lett. 90 (14) (2007) 143111-1–143111-3. [5] R. Nandkishore, L. Levitov, Proc. Natl. Acad. Sci. 108 (2011) 14021–14025. [6] Pei Zhao, R. M. Feenstraz, G. Gu, et al., arXiv:1301.0673. [7] M. Dragoman, A. Dinescu, D. Dragoman, arXiv:1405.6407. [8] P.M. Campbell, A. Tarasov, C.A. Joiner, et al., ACS Nano 9 (5) (2015) 5000–5008. [9] Y.A. Bychkov, E.I. Rashba, J. Phys. C Solid State Phys. 17 (1984) 6039. [10] Goran Isić, et al., J. Appl. Phys. 108 (2010) 044506. [11] David Z.-Y. Ting, et al., Proc. IEEE 91 (2003) 5. [12] Wu Qing-Ping, et al., Appl. Phys. Lett. 105 (2014) 252402. [13] A. Iovan, et al., Nano Lett. 8 (3) (2008) 805–809. [14] H. Mohammadpour, J. Magn. Magn. Mater. 385 (2015) 129–132. [15] H. Mohammadpour, A. Asgari, Phys. E 46 (2012) 270–273. [16] H. Mohammadpour, A. Asgari, Phys. E Low Dimens. Syst. Nanostruct. (2011) 43. [17] R. Grassi, S. Poli, E. Gnani, et al., Solid-State Electron. 53 (2009) 462. [18] R. Grassi, A. Gnudi, S. Reggiani, et al., J. Comput. Electron. 8 (2009) 441. [19] K.I. Bolotin, K.J. Sikes, Z. Zhang, et al., Solid State Commun. 146 (9/10) (2008) 351. [20] M.P. Lopez Sancho, J.M. Lopez Sancho, J. Rubio, J. Phys. F (1985) 15.

Copyright © 2022 COEK.INFO. All rights reserved.